#------------------------------------------------------------------------------
#$Date: 2019-11-23 12:03:07 +0200 (Sat, 23 Nov 2019) $
#$Revision: 233208 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/23/56/7235657.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7235657
loop_
_publ_author_name
'Saini, Mukesh Kumar'
'Gupta, Rakesh'
'Parbhakar, Swati'
'Kumar Mishra, Anil'
'Mathur, Rashi'
'Hussain, Firasat'
_publ_section_title
;
 Dimeric complexes of rare-earth substituted Keggin-type silicotungstates:
 syntheses, crystal structure and solid state properties
;
_journal_issue                   48
_journal_name_full               'RSC Adv.'
_journal_page_first              25357
_journal_paper_doi               10.1039/C4RA02751E
_journal_volume                  4
_journal_year                    2014
_chemical_formula_moiety         '0.5(C8 Dy4 K16 Na8 O208 Si4 W44), 6(O)'
_chemical_formula_sum            'C4 Dy2 K8 Na4 O110 Si2 W22'
_chemical_formula_weight         6638.41
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_Int_Tables_number      14
_audit_creation_date             2014-03-27
_audit_creation_method
;
Olex2 1.2
(compiled 2014.03.20 svn.r2914 for OlexSys, GUI svn.r4813)
;
_cell_angle_alpha                90
_cell_angle_beta                 110.769(4)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   20.1061(7)
_cell_length_b                   12.6303(3)
_cell_length_c                   21.1101(7)
_cell_measurement_reflns_used    14075
_cell_measurement_temperature    149.9
_cell_measurement_theta_max      29.8076
_cell_measurement_theta_min      2.8898
_cell_volume                     5012.5(3)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
;
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'olex2.refine (Bourhis et al., 2013)'
_diffrn_ambient_temperature      149.9
_diffrn_detector_area_resol_mean 15.9853
_diffrn_measured_fraction_theta_full 0.9986
_diffrn_measured_fraction_theta_max 0.9986
_diffrn_measurement_device_type  'Xcalibur, Sapphire3'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_UB_11      0.0159416000
_diffrn_orient_matrix_UB_12      0.0286121000
_diffrn_orient_matrix_UB_13      0.0305807000
_diffrn_orient_matrix_UB_21      0.0329013000
_diffrn_orient_matrix_UB_22      -0.0000411000
_diffrn_orient_matrix_UB_23      -0.0053863000
_diffrn_orient_matrix_UB_31      -0.0093921000
_diffrn_orient_matrix_UB_32      0.0482843000
_diffrn_orient_matrix_UB_33      -0.0180786000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0917
_diffrn_reflns_av_unetI/netI     0.0789
_diffrn_reflns_limit_h_max       25
_diffrn_reflns_limit_h_min       -28
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            75690
_diffrn_reflns_theta_full        26.0208
_diffrn_reflns_theta_max         26.02
_diffrn_reflns_theta_min         2.90
_diffrn_source                   'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    27.095
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.27418
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'clear colourless'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    4.3982
_exptl_crystal_description       'rect. Prism'
_exptl_crystal_F_000             5759.3086
_exptl_crystal_size_max          0.11
_exptl_crystal_size_mid          0.11
_exptl_crystal_size_min          0.03
_refine_diff_density_max         9.3106
_refine_diff_density_min         -3.4613
_refine_diff_density_rms         0.7513
_refine_ls_d_res_high            0.8100
_refine_ls_d_res_low             7.0345
_refine_ls_goodness_of_fit_ref   1.0515
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     389
_refine_ls_number_reflns         9866
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.0515
_refine_ls_R_factor_all          0.0650
_refine_ls_R_factor_gt           0.0515
_refine_ls_shift/su_max          0.0006
_refine_ls_shift/su_mean         0.0000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0268P)²+309.1990P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1015
_refine_ls_wR_factor_ref         0.1074
_reflns_Friedel_coverage         0.0
_reflns_limit_h_max              23
_reflns_limit_h_min              -24
_reflns_limit_k_max              15
_reflns_limit_k_min              0
_reflns_limit_l_max              26
_reflns_limit_l_min              0
_reflns_number_gt                8396
_reflns_number_total             9866
_reflns_threshold_expression     I>=2u(I)
_cod_data_source_file            c4ra02751e2.cif
_cod_data_source_block           fhms-23-4
_cod_database_code               7235657
_chemical_oxdiff_usercomment     '26 DEC 2013'
_reflns_odcompleteness_completeness 99.80
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     26.32
_olex2_refinement_description
;
;
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,y+1/2,-z+1/2
3 -x,-y,-z
4 x,-y-1/2,z-1/2
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
C1 C -0.1346(10) 1.0828(14) 0.0711(9) 0.017(4) Uiso 1.000000
C2 C -0.0772(9) 1.0110(13) 0.0664(8) 0.011(4) Uiso 1.000000
O1 O 0.4946(7) 0.8713(10) 0.4339(6) 0.019(3) Uiso 1.000000
O2 O 0.4244(7) 0.5760(9) 0.2250(6) 0.015(3) Uiso 1.000000
O3 O 0.2917(7) 0.5636(9) 0.4093(6) 0.015(3) Uiso 1.000000
O4 O 0.4437(6) 0.7449(9) 0.3186(6) 0.013(3) Uiso 1.000000
O5 O 0.3484(7) 0.5967(9) 0.3109(6) 0.013(3) Uiso 1.000000
O6 O 0.3770(7) 0.7388(9) 0.4095(6) 0.014(3) Uiso 1.000000
O7 O 0.4184(6) 0.9545(9) 0.3050(6) 0.010(2) Uiso 1.000000
O8 O 0.3838(6) 0.7875(8) 0.1880(5) 0.009(2) Uiso 1.000000
O9 O 0.2864(7) 0.6458(9) 0.1778(6) 0.015(3) Uiso 1.000000
O10 O 0.2079(6) 0.6347(9) 0.2832(6) 0.013(3) Uiso 1.000000
O11 O 0.2377(6) 0.7716(9) 0.3820(6) 0.012(3) Uiso 1.000000
O12 O 0.3528(6) 0.9457(8) 0.3926(5) 0.009(2) Uiso 1.000000
O13 O 0.3099(6) 0.7932(8) 0.2855(5) 0.005(2) Uiso 1.000000
O14 O 0.1166(7) 0.8414(9) 0.4076(6) 0.015(3) Uiso 1.000000
O15 O 0.2301(7) 0.9746(9) 0.4101(6) 0.015(3) Uiso 1.000000
O16 O 0.3244(7) 1.1465(10) 0.4371(6) 0.019(3) Uiso 1.000000
O17 O 0.3279(7) 1.1018(9) 0.3058(6) 0.014(3) Uiso 1.000000
O18 O 0.4437(7) 1.1639(9) 0.2727(6) 0.015(3) Uiso 1.000000
O19 O 0.4025(7) 0.9948(9) 0.1777(6) 0.016(3) Uiso 1.000000
O20 O 0.3804(6) 0.8668(9) 0.0643(6) 0.014(3) Uiso 1.000000
O21 O 0.2600(6) 0.7976(8) 0.0896(5) 0.008(2) Uiso 1.000000
O22 O 0.2031(7) 0.6005(9) 0.0456(6) 0.016(3) Uiso 1.000000
O23 O 0.1449(6) 0.6093(9) 0.1469(6) 0.011(2) Uiso 1.000000
O24 O 0.0657(7) 0.5788(9) 0.2295(6) 0.016(3) Uiso 1.000000
O25 O 0.1158(6) 0.7813(9) 0.2819(6) 0.013(3) Uiso 1.000000
O26 O 0.2151(6) 0.9433(8) 0.2830(5) 0.008(2) Uiso 1.000000
O27 O 0.2819(6) 0.9495(8) 0.1945(5) 0.009(2) Uiso 1.000000
O28 O 0.1862(6) 0.7964(8) 0.1848(5) 0.008(2) Uiso 1.000000
O29 O 0.1040(6) 0.9898(8) 0.3093(5) 0.009(2) Uiso 1.000000
O30 O 0.2024(6) 1.1335(9) 0.3219(6) 0.012(3) Uiso 1.000000
O31 O 0.3096(6) 1.1457(9) 0.1776(6) 0.011(2) Uiso 1.000000
O32 O 0.2789(6) 1.0081(9) 0.0766(6) 0.011(2) Uiso 1.000000
O33 O 0.1148(6) 0.7598(9) 0.0490(6) 0.013(3) Uiso 1.000000
O34 O 0.0433(6) 0.7538(8) 0.1483(5) 0.008(2) Uiso 1.000000
O35 O 0.1470(6) 0.9826(9) 0.0866(6) 0.011(2) Uiso 1.000000
O36 O 0.0758(6) 0.9813(9) 0.1757(6) 0.013(3) Uiso 1.000000
O37 O 0.1847(6) 1.1169(9) 0.1908(5) 0.010(2) Uiso 1.000000
O38 O 0.0676(7) 1.1772(9) 0.2293(6) 0.015(3) Uiso 1.000000
O39 O 0.1864(6) 1.1808(9) 0.0611(6) 0.013(3) Uiso 1.000000
O40 O 0.0334(6) 0.9572(9) -0.0380(6) 0.011(2) Uiso 1.000000
O41 O -0.0419(6) 0.7794(9) -0.0038(6) 0.013(3) Uiso 1.000000
O42 O -0.0683(7) 0.9202(9) 0.0923(6) 0.017(3) Uiso 1.000000
O43 O -0.1735(8) 0.8976(11) 0.1830(7) 0.029(3) Uiso 1.000000
O44 O 0.4579(10) 0.9005(14) 0.5856(9) 0.053(5) Uiso 1.000000
O45 O 0.3928(8) 0.3855(11) 0.3202(7) 0.032(4) Uiso 1.000000
O46 O 0.0762(9) 1.3742(12) -0.0979(8) 0.040(4) Uiso 1.000000
O47 O 0.4683(12) 1.2921(17) 0.4442(11) 0.074(6) Uiso 1.000000
O48 O 0.3151(6) 1.3766(9) 0.4817(6) 0.011(2) Uiso 1.000000
O49 O 0.4723(8) 1.4061(11) 0.5942(7) 0.028(3) Uiso 1.000000
O50 O 0.3682(9) 1.2001(12) 0.6125(8) 0.037(4) Uiso 1.000000
O51 O 0.2273(8) 1.3847(11) 0.0299(7) 0.030(3) Uiso 1.000000
O52 O 0.1635(9) 1.3975(13) 0.1306(8) 0.041(4) Uiso 1.000000
O53 O -0.0295(9) 0.8071(12) 0.3826(8) 0.040(4) Uiso 1.000000
O54 O 0.2551(8) 1.3174(11) 0.2482(7) 0.029(3) Uiso 1.000000
O55 O 0.0505(6) 0.5377(9) -0.0188(6) 0.013(3) Uiso 1.000000
Na1 Na 0.4528(6) 0.9462(8) -0.0125(5) 0.046(2) Uiso 1.000000
Na2 Na 0.4056(5) 1.2552(7) 0.5212(4) 0.034(2) Uiso 1.000000
Si1 Si 0.2473(3) 0.8695(4) 0.2358(2) 0.0086(9) Uani 1.000000
K1 K -0.0275(2) 0.8809(3) 0.23142(19) 0.0162(8) Uani 1.000000
K2 K 0.3272(3) 0.8409(4) 0.5107(2) 0.0276(11) Uani 1.000000
K3 K 0.4718(2) 0.3678(3) 0.2384(2) 0.0182(9) Uani 1.000000
K4 K 0.1889(3) 1.2374(4) -0.0688(2) 0.0341(12) Uani 1.000000
Dy1 Dy 0.04553(4) 0.88871(6) 0.07341(4) 0.00877(17) Uani 1.000000
W1 W 0.41412(4) 0.84889(5) 0.37013(3) 0.00972(15) Uani 1.000000
W2 W 0.37122(4) 0.67006(5) 0.24087(3) 0.00976(15) Uani 1.000000
W3 W 0.28908(4) 0.66310(5) 0.35402(3) 0.00982(15) Uani 1.000000
W4 W 0.16249(4) 0.87299(5) 0.35494(3) 0.00887(15) Uani 1.000000
W5 W 0.28524(4) 1.06036(5) 0.37103(3) 0.00958(15) Uani 1.000000
W6 W 0.37720(4) 1.07174(5) 0.24676(3) 0.00869(15) Uani 1.000000
W7 W 0.33834(4) 0.89212(5) 0.12133(3) 0.00891(15) Uani 1.000000
W8 W 0.19316(4) 0.69593(5) 0.09979(3) 0.00898(15) Uani 1.000000
W9 W 0.11218(4) 0.68110(5) 0.21076(3) 0.00878(15) Uani 1.000000
W10 W 0.21584(4) 1.07658(5) 0.11760(3) 0.00837(15) Uani 1.000000
W11 W 0.12531(4) 1.07119(5) 0.23937(3) 0.00827(15) Uani 1.000000
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
_atom_type_scat_dispersion_source
C 0.00347 0.00161 2.31000 1.02000 1.58860 0.86500 20.84390 10.20750 0.56870
51.65120 0.215599998832
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Na 0.03665 0.02467 4.76260 3.17360 1.26740 1.11280 3.28500 8.84220 0.31360
129.42400 0.675999999046
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
K 0.21174 0.26561 8.21860 7.43980 1.05190 0.86590 12.79490 0.77480 213.18700
41.68410 1.42279994488
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
O 0.01158 0.00611 3.04850 2.28680 1.54630 0.86700 13.27710 5.70110 0.32390
32.90890 0.250800013542
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Si 0.08192 0.07060 6.29150 3.03530 1.98910 1.54100 2.43860 32.33370 0.67850
81.69370 1.14069998264
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
W -0.66836 6.76498 29.08180 15.43000 14.43270 5.11982 1.72029 9.22590 0.32170
57.05600 9.88749980927
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Dy -0.09334 4.42894 26.50700 17.63830 14.55960 2.96577 2.18020 0.20217 12.18990
111.87400 4.29727983475
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O40 C2 C1 120.6(15) 3_575 .
O42 C2 C1 121.2(16) . .
O42 C2 O40 118.1(15) . 3_575
Dy1 C2 C1 172.1(12) . .
Dy1 C2 O40 58.4(8) . 3_575
Dy1 C2 O42 59.9(9) . .
W1 O1 Na2 127.0(6) . 3_676
W2 O2 K3 148.7(6) . .
W1 O4 K3 102.4(5) . 2_655
W2 O4 K3 106.2(5) . 2_655
W2 O4 W1 120.2(6) . .
W3 O5 W2 120.4(6) . .
W1 O6 K2 106.4(5) . .
W3 O6 K2 100.3(5) . .
W3 O6 W1 119.9(6) . .
W1 O7 K3 101.3(4) . 2_655
W6 O7 K3 107.1(5) . 2_655
W6 O7 W1 150.3(7) . .
W2 O8 K3 105.5(4) . 2_655
W7 O8 K3 105.9(4) . 2_655
W7 O8 W2 146.4(7) . .
W8 O9 W2 152.2(7) . .
W9 O10 W3 151.6(6) . .
W3 O11 K2 106.7(5) . .
W4 O11 K2 104.3(5) . .
W4 O11 W3 146.9(6) . .
W1 O12 K2 103.8(4) . .
W5 O12 K2 102.2(4) . .
W5 O12 W1 152.3(6) . .
W1 O13 Si1 126.4(6) . .
W2 O13 Si1 121.3(5) . .
W2 O13 W1 92.8(4) . .
W3 O13 Si1 123.2(6) . .
W3 O13 W1 92.8(4) . .
W3 O13 W2 91.0(4) . .
W4 O15 K2 101.7(5) . .
W5 O15 K2 107.7(5) . .
W5 O15 W4 120.3(6) . .
K4 O16 Na2 96.8(5) 4_586 .
W5 O16 Na2 164.8(8) . .
W5 O16 K4 97.2(5) . 4_586
W6 O17 W5 152.3(7) . .
W6 O18 K3 138.9(6) . 1_565
W6 O19 K3 102.3(5) . 2_655
W7 O19 K3 104.3(5) . 2_655
W7 O19 W6 120.1(6) . .
K2 O20 Na1 107.5(4) 4_575 .
W7 O20 Na1 147.4(6) . .
W7 O20 K2 103.6(5) . 4_575
W7 O21 K2 94.7(4) . 4_575
W8 O21 K2 98.1(4) . 4_575
W8 O21 W7 154.7(6) . .
W8 O22 K2 107.4(5) . 4_575
W9 O23 W8 116.6(6) . .
W9 O24 K1 163.4(7) . 2_545
W4 O25 K1 99.9(5) . .
W9 O25 K1 103.4(5) . .
W9 O25 W4 154.1(7) . .
W4 O26 Si1 123.1(6) . .
W5 O26 Si1 124.4(6) . .
W5 O26 W4 90.5(4) . .
W11 O26 Si1 124.1(6) . .
W11 O26 W4 93.1(4) . .
W11 O26 W5 92.2(4) . .
W6 O27 Si1 124.8(6) . .
W7 O27 Si1 123.9(6) . .
W7 O27 W6 90.4(4) . .
W10 O27 Si1 123.3(6) . .
W10 O27 W6 92.4(4) . .
W10 O27 W7 92.5(4) . .
W8 O28 Si1 127.7(6) . .
W9 O28 Si1 127.9(6) . .
W9 O28 W8 93.6(4) . .
W4 O29 K1 101.1(4) . .
W11 O29 K1 102.6(4) . .
W11 O29 W4 121.4(6) . .
W5 O30 K4 98.7(4) . 4_586
W11 O30 K4 129.7(5) . 4_586
W11 O30 W5 122.9(6) . .
W10 O31 W6 121.8(6) . .
W10 O32 W7 120.4(6) . .
W8 O33 Dy1 131.9(6) . .
Dy1 O34 K1 97.4(4) . .
W9 O34 K1 104.0(4) . .
W9 O34 Dy1 132.6(6) . .
W10 O35 Dy1 160.4(6) . .
Dy1 O36 K1 99.2(4) . .
W11 O36 K1 104.7(5) . .
W11 O36 Dy1 156.0(7) . .
W11 O37 W10 142.1(6) . .
W11 O38 K1 152.9(6) . 2
W10 O39 K4 137.2(6) . .
Dy1 O40 C2 94.9(9) 3_575 3_575
Dy1 O40 C2 135.0(11) . 3_575
K1 O42 C2 124.2(10) . .
K4 O42 C2 123.0(11) 3_575 .
K4 O42 K1 88.6(4) 3_575 .
Dy1 O42 C2 94.2(10) . .
Dy1 O42 K1 101.3(4) . .
Dy1 O42 K4 126.5(5) . 3_575
K4 O43 K1 92.9(4) 3_575 .
Na2 O47 Na1 97.6(8) . 2_655
K4 O48 Na2 106.9(5) 4_586 .
Na2 O49 Na1 92.8(5) . 2_655
K3 O50 Na2 119.9(7) 4_576 .
O47 Na1 O20 75.2(6) 2_645 .
O49 Na1 O20 147.6(5) 2_645 .
O49 Na1 O47 81.1(6) 2_645 2_645
Na1 Na1 O20 132.1(7) 3_675 .
Na1 Na1 O47 91.4(8) 3_675 2_645
Na1 Na1 O49 69.4(6) 3_675 2_645
O16 Na2 O1 99.3(5) . 3_676
O47 Na2 O1 80.6(7) . 3_676
O47 Na2 O16 89.6(7) . .
O48 Na2 O1 178.2(6) . 3_676
O48 Na2 O16 82.5(5) . .
O48 Na2 O47 99.2(7) . .
O49 Na2 O1 94.1(5) . 3_676
O49 Na2 O16 166.0(6) . .
O49 Na2 O47 88.5(7) . .
O49 Na2 O48 84.2(5) . .
O50 Na2 O1 87.0(5) . 3_676
O50 Na2 O16 96.0(6) . .
O50 Na2 O47 167.1(8) . .
O50 Na2 O48 93.0(6) . .
O50 Na2 O49 88.8(6) . .
O26 Si1 O13 108.8(6) . .
O27 Si1 O13 109.2(6) . .
O27 Si1 O26 107.6(6) . .
O28 Si1 O13 108.8(6) . .
O28 Si1 O26 111.0(6) . .
O28 Si1 O27 111.4(6) . .
O25 K1 O24 126.8(4) . 2
O29 K1 O24 72.8(3) . 2
O29 K1 O25 55.1(3) . .
O34 K1 O24 149.2(3) . 2
O34 K1 O25 53.0(3) . .
O34 K1 O29 93.3(3) . .
O36 K1 O24 92.2(3) . 2
O36 K1 O25 66.6(3) . .
O36 K1 O29 53.7(3) . .
O36 K1 O34 58.2(3) . .
O38 K1 O24 124.7(4) 2_545 2
O38 K1 O25 81.6(3) 2_545 .
O38 K1 O29 123.0(3) 2_545 .
O38 K1 O34 86.0(3) 2_545 .
O38 K1 O36 141.8(4) 2_545 .
O42 K1 O24 98.1(4) . 2
O42 K1 O25 109.7(4) . .
O42 K1 O29 112.2(4) . .
O42 K1 O34 61.1(3) . .
O42 K1 O36 60.1(3) . .
O42 K1 O38 116.6(4) . 2_545
O43 K1 O24 71.1(4) . 2
O43 K1 O25 159.3(4) . .
O43 K1 O29 143.9(4) . .
O43 K1 O34 118.4(4) . .
O43 K1 O36 128.0(4) . .
O43 K1 O38 78.8(4) . 2_545
O43 K1 O42 73.7(4) . .
O53 K1 O24 82.6(4) . 2
O53 K1 O25 83.0(4) . .
O53 K1 O29 84.7(4) . .
O53 K1 O34 124.4(4) . .
O53 K1 O36 137.4(4) . .
O53 K1 O38 51.8(4) . 2_545
O53 K1 O42 162.5(4) . .
O53 K1 O43 90.2(4) . .
O11 K2 O6 55.3(3) . .
O12 K2 O6 52.8(3) . .
O12 K2 O11 65.0(3) . .
O15 K2 O6 92.1(3) . .
O15 K2 O11 55.5(3) . .
O15 K2 O12 53.3(3) . .
O20 K2 O6 73.5(3) 4_576 .
O20 K2 O11 96.6(4) 4_576 .
O20 K2 O12 124.7(3) 4_576 .
O20 K2 O15 151.5(4) 4_576 .
O21 K2 O6 118.3(3) 4_576 .
O21 K2 O11 95.4(3) 4_576 .
O21 K2 O12 160.3(3) 4_576 .
O21 K2 O15 115.3(4) 4_576 .
O21 K2 O20 56.0(3) 4_576 4_576
O22 K2 O6 145.8(4) 4_576 .
O22 K2 O11 90.7(4) 4_576 .
O22 K2 O12 120.3(3) 4_576 .
O22 K2 O15 67.8(3) 4_576 .
O22 K2 O20 111.0(4) 4_576 4_576
O22 K2 O21 55.0(3) 4_576 4_576
O44 K2 O6 92.1(5) . .
O44 K2 O11 145.4(5) . .
O44 K2 O12 86.8(5) . .
O44 K2 O15 123.0(5) . .
O44 K2 O20 82.7(5) . 4_576
O44 K2 O21 112.0(5) . 4_576
O44 K2 O22 122.0(5) . 4_576
O4 K3 O2 134.8(4) 2_645 .
O7 K3 O2 83.2(3) 2_645 .
O7 K3 O4 55.8(3) 2_645 2_645
O8 K3 O2 128.2(4) 2_645 .
O8 K3 O4 54.1(3) 2_645 2_645
O8 K3 O7 65.0(3) 2_645 2_645
O18 K3 O2 143.8(4) 1_545 .
O18 K3 O4 79.2(4) 1_545 2_645
O18 K3 O7 132.9(4) 1_545 2_645
O18 K3 O8 78.3(3) 1_545 2_645
O19 K3 O2 74.9(4) 2_645 .
O19 K3 O4 92.1(4) 2_645 2_645
O19 K3 O7 53.4(3) 2_645 2_645
O19 K3 O8 53.4(3) 2_645 2_645
O19 K3 O18 123.3(4) 2_645 1_545
O45 K3 O2 74.5(4) . .
O45 K3 O4 150.8(4) . 2_645
O45 K3 O7 148.0(4) . 2_645
O45 K3 O8 112.3(4) . 2_645
O45 K3 O18 72.3(4) . 1_545
O45 K3 O19 98.1(4) . 2_645
O50 K3 O2 94.5(4) 4_575 .
O50 K3 O4 78.0(4) 4_575 2_645
O50 K3 O7 101.8(4) 4_575 2_645
O50 K3 O8 130.0(4) 4_575 2_645
O50 K3 O18 79.4(4) 4_575 1_545
O50 K3 O19 153.5(4) 4_575 2_645
O50 K3 O45 102.4(5) 4_575 .
O30 K4 O16 55.4(3) 4_585 4_585
O39 K4 O16 113.6(4) . 4_585
O39 K4 O30 160.0(4) . 4_585
O42 K4 O16 165.6(4) 3_575 4_585
O42 K4 O30 122.0(4) 3_575 4_585
O42 K4 O39 73.0(3) 3_575 .
O43 K4 O16 98.5(4) 3_575 4_585
O43 K4 O30 71.4(4) 3_575 4_585
O43 K4 O39 128.6(4) 3_575 .
O43 K4 O42 68.4(4) 3_575 3_575
O46 K4 O16 111.2(4) . 4_585
O46 K4 O30 76.8(4) . 4_585
O46 K4 O39 94.5(4) . .
O46 K4 O42 80.1(4) . 3_575
O46 K4 O43 110.5(5) . 3_575
O48 K4 O16 63.5(3) 4_585 4_585
O48 K4 O30 105.4(4) 4_585 4_585
O48 K4 O39 80.0(4) 4_585 .
O48 K4 O42 106.9(4) 4_585 3_575
O48 K4 O43 80.0(4) 4_585 3_575
O48 K4 O46 169.2(5) 4_585 .
O51 K4 O16 68.3(4) . 4_585
O51 K4 O30 98.3(4) . 4_585
O51 K4 O39 61.8(4) . .
O51 K4 O42 124.9(4) . 3_575
O51 K4 O43 166.7(5) . 3_575
O51 K4 O46 74.1(5) . .
O51 K4 O48 95.1(4) . 4_585
O33 Dy1 C2 160.1(4) . .
O34 Dy1 C2 101.8(4) . .
O34 Dy1 O33 78.2(4) . .
O35 Dy1 C2 116.2(4) . .
O35 Dy1 O33 79.1(4) . .
O35 Dy1 O34 121.7(4) . .
O36 Dy1 C2 73.5(4) . .
O36 Dy1 O33 125.2(4) . .
O36 Dy1 O34 78.5(4) . .
O36 Dy1 O35 72.5(4) . .
O40 Dy1 C2 26.7(4) 3_575 .
O40 Dy1 C2 88.3(4) . .
O40 Dy1 O33 149.9(4) 3_575 .
O40 Dy1 O33 84.1(4) . .
O40 Dy1 O34 128.2(4) 3_575 .
O40 Dy1 O34 153.3(4) . .
O40 Dy1 O35 94.5(4) 3_575 .
O40 Dy1 O35 73.4(4) . .
O40 Dy1 O36 128.2(4) . .
O40 Dy1 O36 79.2(4) 3_575 .
O41 Dy1 C2 82.1(4) . .
O41 Dy1 O33 78.2(4) . .
O41 Dy1 O34 81.5(4) . .
O41 Dy1 O35 142.9(4) . .
O41 Dy1 O36 144.3(4) . .
O41 Dy1 O40 90.6(4) . 3_575
O41 Dy1 O40 75.4(4) . .
O42 Dy1 C2 25.9(4) . .
O42 Dy1 O33 143.8(4) . .
O42 Dy1 O34 76.6(4) . .
O42 Dy1 O35 136.7(4) . .
O42 Dy1 O36 74.1(4) . .
O42 Dy1 O40 108.4(4) . .
O42 Dy1 O40 52.4(4) . 3_575
O42 Dy1 O41 72.7(4) . .
O4 W1 O1 99.3(5) . .
O6 W1 O1 100.6(5) . .
O6 W1 O4 89.8(5) . .
O7 W1 O1 100.1(5) . .
O7 W1 O4 88.2(5) . .
O7 W1 O6 159.2(5) . .
O12 W1 O1 102.2(5) . .
O12 W1 O4 158.4(5) . .
O12 W1 O6 88.3(5) . .
O12 W1 O7 86.0(5) . .
O13 W1 O1 171.8(5) . .
O13 W1 O4 74.6(4) . .
O13 W1 O6 74.2(4) . .
O13 W1 O7 85.3(4) . .
O13 W1 O12 84.2(4) . .
O4 W2 O2 99.5(5) . .
O5 W2 O2 98.7(5) . .
O5 W2 O4 84.3(5) . .
O8 W2 O2 101.7(5) . .
O8 W2 O4 84.5(5) . .
O8 W2 O5 158.1(5) . .
O9 W2 O2 103.6(6) . .
O9 W2 O4 156.9(5) . .
O9 W2 O5 93.7(5) . .
O9 W2 O8 89.2(5) . .
O13 W2 O2 168.8(5) . .
O13 W2 O4 72.2(4) . .
O13 W2 O5 73.3(4) . .
O13 W2 O8 85.4(4) . .
O13 W2 O9 85.1(5) . .
O5 W3 O3 97.4(5) . .
O6 W3 O3 98.4(5) . .
O6 W3 O5 85.3(5) . .
O10 W3 O3 102.6(5) . .
O10 W3 O5 92.9(5) . .
O10 W3 O6 158.9(5) . .
O11 W3 O3 101.7(5) . .
O11 W3 O5 160.1(5) . .
O11 W3 O6 86.5(5) . .
O11 W3 O10 88.3(5) . .
O13 W3 O3 168.6(5) . .
O13 W3 O5 74.7(4) . .
O13 W3 O6 73.0(4) . .
O13 W3 O10 86.3(4) . .
O13 W3 O11 85.5(4) . .
O14 W4 O11 101.5(5) . .
O15 W4 O11 87.3(5) . .
O15 W4 O14 100.9(5) . .
O25 W4 O11 86.8(5) . .
O25 W4 O14 99.2(5) . .
O25 W4 O15 159.8(5) . .
O26 W4 O11 87.5(4) . .
O26 W4 O14 170.3(5) . .
O26 W4 O15 75.7(4) . .
O26 W4 O25 84.8(4) . .
O29 W4 O11 161.0(5) . .
O29 W4 O14 97.4(5) . .
O29 W4 O15 88.1(5) . .
O29 W4 O25 91.3(5) . .
O29 W4 O26 73.6(4) . .
O15 W5 O12 86.6(5) . .
O16 W5 O12 101.7(5) . .
O16 W5 O15 100.1(5) . .
O17 W5 O12 85.3(5) . .
O17 W5 O15 157.2(5) . .
O17 W5 O16 102.4(5) . .
O26 W5 O12 83.7(4) . .
O26 W5 O15 73.5(4) . .
O26 W5 O16 171.6(5) . .
O26 W5 O17 84.4(4) . .
O30 W5 O12 156.9(5) . .
O30 W5 O15 88.9(5) . .
O30 W5 O16 101.5(5) . .
O30 W5 O17 90.2(5) . .
O30 W5 O26 73.2(4) . .
O17 W6 O7 86.6(5) . .
O18 W6 O7 102.1(5) . .
O18 W6 O17 100.7(5) . .
O19 W6 O7 85.8(5) . .
O19 W6 O17 157.8(5) . .
O19 W6 O18 101.3(5) . .
O27 W6 O7 83.7(4) . .
O27 W6 O17 84.9(4) . .
O27 W6 O18 172.0(5) . .
O27 W6 O19 73.5(4) . .
O31 W6 O7 157.5(5) . .
O31 W6 O17 90.5(5) . .
O31 W6 O18 100.4(5) . .
O31 W6 O19 88.6(5) . .
O31 W6 O27 73.7(4) . .
O19 W7 O8 88.3(5) . .
O20 W7 O8 99.3(5) . .
O20 W7 O19 99.8(5) . .
O21 W7 O8 86.9(5) . .
O21 W7 O19 159.4(5) . .
O21 W7 O20 100.8(5) . .
O27 W7 O8 86.8(4) . .
O27 W7 O19 75.9(5) . .
O27 W7 O20 172.5(5) . .
O27 W7 O21 83.8(4) . .
O32 W7 O8 160.8(5) . .
O32 W7 O19 87.3(5) . .
O32 W7 O20 99.9(5) . .
O32 W7 O21 90.7(5) . .
O32 W7 O27 74.0(4) . .
O21 W8 O9 79.9(5) . .
O22 W8 O9 91.6(5) . .
O22 W8 O21 98.2(5) . .
O23 W8 O9 84.2(5) . .
O23 W8 O21 157.4(5) . .
O23 W8 O22 98.2(5) . .
O28 W8 O9 80.5(4) . .
O28 W8 O21 87.5(4) . .
O28 W8 O22 169.4(5) . .
O28 W8 O23 74.1(4) . .
O33 W8 O9 166.4(5) . .
O33 W8 O21 97.8(5) . .
O33 W8 O22 101.9(5) . .
O33 W8 O23 93.9(5) . .
O33 W8 O28 86.1(5) . .
O23 W9 O10 85.7(5) . .
O24 W9 O10 93.2(5) . .
O24 W9 O23 99.0(5) . .
O25 W9 O10 81.0(5) . .
O25 W9 O23 156.8(5) . .
O25 W9 O24 100.7(5) . .
O28 W9 O10 81.0(4) . .
O28 W9 O23 73.7(4) . .
O28 W9 O24 170.9(5) . .
O28 W9 O25 85.5(4) . .
O34 W9 O10 164.1(5) . .
O34 W9 O23 95.4(5) . .
O34 W9 O24 102.3(5) . .
O34 W9 O25 92.4(5) . .
O34 W9 O28 84.1(5) . .
O31 W10 O27 72.1(4) . .
O32 W10 O27 73.0(4) . .
O32 W10 O31 82.2(5) . .
O35 W10 O27 88.4(5) . .
O35 W10 O31 160.3(5) . .
O35 W10 O32 94.8(5) . .
O37 W10 O27 83.7(4) . .
O37 W10 O31 83.2(5) . .
O37 W10 O32 155.4(5) . .
O37 W10 O35 92.3(5) . .
O39 W10 O27 166.5(5) . .
O39 W10 O31 96.7(5) . .
O39 W10 O32 98.5(5) . .
O39 W10 O35 103.0(5) . .
O39 W10 O37 102.8(5) . .
O29 W11 O26 71.8(4) . .
O30 W11 O26 71.6(4) . .
O30 W11 O29 82.0(5) . .
O36 W11 O26 90.2(5) . .
O36 W11 O29 91.2(5) . .
O36 W11 O30 161.8(5) . .
O37 W11 O26 83.1(4) . .
O37 W11 O29 154.3(5) . .
O37 W11 O30 85.0(5) . .
O37 W11 O36 94.4(5) . .
O38 W11 O26 164.7(5) . .
O38 W11 O29 100.4(5) . .
O38 W11 O30 94.5(5) . .
O38 W11 O36 103.3(5) . .
O38 W11 O37 102.6(5) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
C1 C2 1.50(2) .
C2 O40 1.29(2) 3_575
C2 O42 1.26(2) .
C2 Dy1 2.870(17) .
O1 Na2 2.476(15) 3_676
O1 W1 1.722(13) .
O2 K3 2.776(12) .
O2 W2 1.709(12) .
O3 W3 1.703(12) .
O4 K3 2.864(12) 2_655
O4 W1 1.929(11) .
O4 W2 2.003(12) .
O5 W2 1.934(12) .
O5 W3 1.929(12) .
O6 K2 2.958(13) .
O6 W1 1.903(12) .
O6 W3 1.985(12) .
O7 K3 2.888(12) 2_655
O7 W1 1.940(11) .
O7 W6 1.915(11) .
O8 K3 2.944(12) 2_655
O8 W2 1.926(11) .
O8 W7 1.911(11) .
O9 W2 1.778(12) .
O9 W8 2.107(12) .
O10 W3 1.817(12) .
O10 W9 2.073(12) .
O11 K2 2.814(12) .
O11 W3 1.930(12) .
O11 W4 1.908(12) .
O12 K2 3.025(11) .
O12 W1 1.912(11) .
O12 W5 1.926(11) .
O13 Si1 1.637(11) .
O13 W1 2.328(11) .
O13 W2 2.378(10) .
O13 W3 2.323(10) .
O14 W4 1.724(12) .
O15 K2 2.869(13) .
O15 W4 1.931(12) .
O15 W5 1.930(12) .
O16 Na2 2.376(15) .
O16 K4 3.057(14) 4_586
O16 W5 1.724(12) .
O17 W5 1.934(12) .
O17 W6 1.887(12) .
O18 K3 2.787(12) 1_565
O18 W6 1.710(12) .
O19 K3 2.986(13) 2_655
O19 W6 1.964(12) .
O19 W7 1.916(12) .
O20 Na1 2.726(16) .
O20 K2 2.907(12) 4_575
O20 W7 1.728(12) .
O21 K2 3.041(12) 4_575
O21 W7 1.898(11) .
O21 W8 1.926(11) .
O22 K2 2.936(13) 4_575
O22 W8 1.721(12) .
O23 W8 1.952(11) .
O23 W9 1.923(11) .
O24 K1 2.822(13) 2_545
O24 W9 1.721(12) .
O25 K1 2.973(13) .
O25 W4 1.890(11) .
O25 W9 1.946(11) .
O26 Si1 1.654(12) .
O26 W4 2.314(11) .
O26 W5 2.402(11) .
O26 W11 2.354(11) .
O27 Si1 1.642(12) .
O27 W6 2.403(11) .
O27 W7 2.334(11) .
O27 W10 2.334(11) .
O28 Si1 1.607(12) .
O28 W8 2.243(11) .
O28 W9 2.283(11) .
O29 K1 2.916(12) .
O29 W4 1.919(11) .
O29 W11 1.967(11) .
O30 K4 2.916(12) 4_586
O30 W5 1.866(12) .
O30 W11 2.035(11) .
O31 W6 1.856(11) .
O31 W10 2.056(12) .
O32 W7 1.915(11) .
O32 W10 1.970(12) .
O33 Dy1 2.315(12) .
O33 W8 1.757(12) .
O34 K1 3.074(12) .
O34 Dy1 2.337(11) .
O34 W9 1.790(11) .
O35 Dy1 2.290(12) .
O35 W10 1.763(11) .
O36 K1 3.006(12) .
O36 Dy1 2.339(11) .
O36 W11 1.771(11) .
O37 W10 1.931(11) .
O37 W11 1.918(11) .
O38 K1 2.904(12) 2
O38 W11 1.735(12) .
O39 K4 2.851(12) .
O39 W10 1.734(11) .
O40 Dy1 2.436(11) .
O40 Dy1 2.455(11) 3_575
O41 Dy1 2.371(12) .
O42 K1 2.799(12) .
O42 K4 3.039(13) 3_575
O42 Dy1 2.491(13) .
O43 K1 2.753(15) .
O43 K4 2.878(15) 3_575
O44 K2 2.651(19) .
O45 K3 2.738(15) .
O46 K4 2.742(17) .
O47 Na1 2.60(2) 2_655
O47 Na2 2.43(2) .
O48 Na2 2.298(14) .
O48 K4 2.779(13) 4_586
O49 Na1 2.709(18) 2_655
O49 Na2 2.517(16) .
O50 Na2 2.405(18) .
O50 K3 2.867(16) 4_576
O51 K4 2.694(15) .
O53 K1 3.339(16) .
Na1 Na1 2.24(2) 3_675
